Ferrihydrite (Fh) is a widespread hydrous ferric oxyhydroxide mineral at the Earth's surface, and a likely constituent in extraterrestrial materials. It forms in several types of environments, from freshwater to marine systems, aquifers to hydrothermal hot springs and scales, soils, and areas affected by mining. It can be precipitated directly from oxygenated iron-rich aqueous solutions, or by bacteria either as a result of a metabolic activity or passive sorption of dissolved iron followed by nucleation reactions. Ferrihydrite also occurs in the core of the ferritin protein from many living organisms, for the purpose of intra-cellular iron storage. Structure Ferrihydrite only exists as a fine grained and highly defective nanomaterial. The powder X-ray diffraction pattern of Fh contains two scattering bands in its most disordered state, and a maximum of six strong lines in its most crystalline state. The principal difference between these two diffraction end-members, commonly named two-line and six-line ferrihydrites, is the size of the constitutive crystallites. The six-line form has been classified as a mineral by the IMA in 1973 with the nominal chemical formula 5•9. Other proposed formulas are •4 and •2•2.6. However, its formula is fundamentally indeterminate as its water content is variable. The two-line form is also called hydrous ferric oxides (HFO). Due to the nanoparticulate nature of ferrihydrite, the structure has remained elusive for many years and is still a matter of controversy. Drits et al., using X-ray diffraction data, proposed in 1993 a multiphase structure model for six-line ferrihydrite with three components: (1) defect-free crystallites (f-phase) with double-hexagonal stacking of oxygen and hydroxyl layers (ABAC sequence) and disordered octahedral Fe occupancies, (2) defective crystallites (d-phase) with a short-range feroxyhite-like (δ-FeOOH) structure, and (3) subordinate ultradisperse hematite (α-Fe2O3). The diffraction model has been confirmed in 2002 by Neutron diffraction, and the three components were observed by High-resolution transmission electron microscopy. A single phase model for both ferrihydrite and hydromaghemite has been proposed by Michel et al., in 2007-2010, based on pair distribution function (PDF) analysis of x-ray total scattering data. The structural model, isostructural with the mineral akdalaite (Al10O14(OH)2), contains 20% tetrahedrally and 80% octahedrally coordinated iron. Manceau et al. showed in 2014 that the Drits et al. model reproduces the PDF data as well as the Michel et al. model. Porosity and environmental absorbent potential Because of the small size of individual nanocrystals, Fh is nanoporous yielding large surface areas of several hundred